Applied IrO2 Buffer Layer as a Great Promoter on Ti-Doping V2O5 Electrode to Enhance Electrochromic Device Properties

Electrochromic devices (ECDs) are a promising material for smart windows that are capable of transmittance variation. However, ECDs are still too expensive to achieve a wide market reach. Reducing fabrication cost remains a challenge. In this study, we inserted an IrO2 buffer layer on Ti-doped V2O5 (Ti:V2O5) as a counter electrode using various Ar/O2 gas flow ratios (1/2, 1/2.5, 1/3 and 1/3.5) in the fabrication process. The buffered-ECD resulted in a larger cyclic voltammetry (CV) area and the best surface average roughness (Ra = 3.91 nm) to promote electrochromic performance. It was fabricated using the low-cost, fast deposition process of vacuum cathodic arc plasma (CAP). This study investigates the influence of the IrO2 buffer/Ti:V2O5 electrode on ECD electrochemical and optical properties, in terms of color efficiency (CE) and cycle durability. The buffered ECD (glass/ITO/WO3/liquid electrolyte/IrO2 buffer/Ti:V2O5/ITO/glass) demonstrated excellent optical transmittance modulation; ∆T = 57% (from Tbleaching (67%) to Tcoloring (10%)) at 633 nm, which was higher than without the buffer (ITO/WO3/liquid electrolyte/Ti:V2O5/ITO) (∆T = 36%). In addition, by means of an IrO2 buffer, the ECD exhibited high coloration efficiency of 96.1 cm2/mC and good durability, which decayed by only 2% after 1000 cycles.


Introduction
As part of the drive to mitigate the global energy crisis, one approach is the development of energy saving devices. Electrochromic devices (ECDs) are regarded as excellent candidates for research, as they feature low power usage, reversible changing, low-power drives large optical modulation, and good memory [1][2][3][4]. ECDs are attracting considerable attention since they have practical applications in smart windows for buildings and in heat-insulating glass for airplanes [5,6].
Smart windows are based on electrochromic materials that block solar and indoor sunlight and heat, enabling a reduction in the energy required for air conditioning [7]. A wide variety of ECD materials have been studied, including transition metal oxides, such as nickel oxide (NiO), tungsten oxide (WO 3 ), zinc oxide (ZnO), and vanadium oxide (V 2 O 5 ) [8][9][10][11].
WO 3 is a well-known cathodic material and NiO is a common anodic material [12][13][14]. The main drawbacks of the NiO ECDs are the low contrast in optical transmittance and short durability [15,16]. Hence, V 2 O 5 film has recently been studied as an anodic electrode in ECD, where it can participate in reversible oxidation and reduction reactions, which facilitate the movement of Li ions into/out of the interface electrodes and electrolyte [17,18]. The typical redox reaction of V 2 O 5 with perchlorate (LiClO 4 ) electrolyte can be written as follows [19]: V 2 O 5 + xLi + + x − = Li x V 2 O 5 (1) investigated in this work. We determined that the buffer is a very important layer in ECD and serves many functions.

Deposition of Ti:V 2 O 5 Counter Electrode and IrO 2 Buffer Layer
The Ti:V 2 O 5 electrode and IrO 2 buffer layer were fabricated by the CAP technique showing in Figure 2 and using the targets of Ti-doped V 2 O 5 (Ti:V = 1:2; 99.95% purity) and metallic iridium (Ir) target (99.95% purity), respectively. We deposited the Ti:V 2 O 5 films (samples 1-4) using a series of reaction Ar/O 2 gas flow ratios (1/2, 1/2.5, 1/3, and 1/3.5) as the counter electrode on indium tin oxide (ITO) glass. The IrO 2 film (sample 5) as the buffer layer with an Ar/O 2 gas flow ratio of 1/3 was stacked on the Ti:V 2 O 5 electrode. The deposition parameters implemented are detailed in Table 1.
investigated in this work. We determined that the buffer is a very important layer i ECD and serves many functions.

Deposition of Ti:V2O5 Counter Electrode and IrO2 Buffer Layer
The Ti:V2O5 electrode and IrO2 buffer layer were fabricated by the CAP techn showing in Figure 2 and using the targets of Ti-doped V2O5 (Ti:V = 1:2; 99.95% purity metallic iridium (Ir) target (99.95% purity), respectively. We deposited the Ti:V2O5 (samples 1-4) using a series of reaction Ar/O2 gas flow ratios (1/2, 1/2.5, 1/3, and 1/3 the counter electrode on indium tin oxide (ITO) glass. The IrO2 film (sample 5) a buffer layer with an Ar/O2 gas flow ratio of 1/3 was stacked on the Ti:V2O5 electrode deposition parameters implemented are detailed in Table 1.   WO 3 working electrodes were produced by an identical CAP method using a metallic tungsten (W) target (99.95% purity) and depositing at fixed Ar/O 2 gas flow ratio of 1/3 on indium tin oxide (ITO) glass substrate (10 × 10 cm 2 ) with resistance of 6 Ω/cm 2 . Cathodic arcs can be used for the reactive deposition of various nitrides and oxides. This can largely be overcome by steering the arc rapidly across the surface of the cathode under high working pressure to reduce the spot residence time and limit the formation of erosion craters [7,38]. In recent years, researchers have shifted the emphasis from monolithic coatings to higher performing multilayers and nanocomposites. In those papers, the proposed arc gun setup relies on the flow of argon (for insertion) and oxygen (reaction) to control the formation of the electrode structure.
During the process, each ITO-coated glass sample prior to deposition was washed with deionized water for 2 min to remove surface-bound particles. For the preparation of the UV-curable poly(methyl methacrylate) (PMMA-based polymer electrolyte, 6.00 g of PMMA monomer) and 0.2 M of LiClO 4 were dissolved in 10.00 g of PC purged by N 2 gas. Afterward, 0.55 g (5 wt%) of IRGACURE 184 and 0.44 g (4 wt%) of phenothiazine were added. The mixture was prepared in a dark vial to avoid exposure to light and was stirred for 12 h period at 60 • C. The multilayer of the ECDs structure was stacked as follows: ITO (300 nm)/Ti:V 2 O 5 (80 nm)/IrO 2 (20 nm)/LiClO 4 PC (100 µm)/WO 3 (200 nm)/ITO (300 nm), which comprised a working electrode (WO 3 film on ITO substrate), a counter-electrode (with or without buffer/Ti:V 2 O 5 /ITO films) in 0.2 M LiClO 4 /PC solution. The processes are detailed in Table 2.

Experimental Details
Scanning of the electrochemical characteristics employed cycle voltammetry (CV) and chronoamperometry (CA) (model PGSTAT30, Autolab, Utrecht, The Netherlands) in a three-electrode system with Ti:V 2 O 5 /ITO/glass and IrO 2 buffer/Ti:V 2 O 5 /ITO/glass as the working electrode, platinum mesh as the counter electrode, and Ag/AgCl as the reference electrode. The film's optical tansmittance in a wavelength range from 300 nm to 900 nm was measured by an ultraviolet-visible (UV-Vis) spectrophotometer (model DH-2000-BAL, Ocean Optics, Dunedin, FL, USA) based on colored/bleached states. The interface roughness topography was collected by atomic force emission (AFM) (model Innova, Bruker, Billerica, MA, USA). The surface and cross-sectional morphology were obtained from scanning emission microscopy (SEM) (Model S4800, Hitachi, Tokyo, Japan) applied at 15 kV. The crystallographic structure was examined by high-resolution X-ray diffractometer (HRXRD, Model D8, Bruker, Billerica, MA, USA) using CuKα (λ = 0.154 nm) as target with a scan region of 20 • to 90 • . Raman spectra were collected by 488 nm laser with an average of 100 scans and a power excitation of 45 mW (Model MOF-iHR550, Horiba, Kyoto, Japan).

Ti:V 2 O 5 /ITO Films: Electrochemical and Optical Properties
Cyclic voltammetry (CV) was implemented to acquire the electrochemical properties of the Ti:V 2 O 5 counter electrode on ITO glass. Figure 3 demonstrates the plot of current density versus potential voltage at the 25th cycle with an applied sweep voltage ranging from −3 V (coloring) to 2.5 V rate (bleaching) and a scan rate of 100 mV/s. The Ti:V 2 O 5 films were processed with various Ar/O 2 gas flow ratios (1/2, 1/2.5, 1/3, and 1/3.5) on ITO glass. However, the Ar/O 2 gas flow ratio of 1/3 resulted a larger enveloped area, indicating that more Li + ions participated in the electrochemical redox reaction [39]. In addition, the CV curve of the Ti:V 2 O 5 films presents two remarkable cathodic reduction peaks (−1.2 V, −1.7 V) and two anodic peaks (−0.75 V, 1.5 V), which were attributed to Li + intercalaltion and Li + extraction, respectively. This higher optical transmittance modulation is a result of the larger CV envelope area on account of the increased number of Li ions into/out of the electrode interface.     (CV) of the 1/3 ratio in Figure 3 and in our previous work [38]. This behavior could be explained by the larger enveloped area and large optical modulation achieved during CV. Electrochromism of the film upon Li + intercalation/extraction was examined by transmittance measurement during the CV process. Considering the highest transmittance (∆T = 27%), we picked an Ar/O 2 gas flow ratio of 1/3 as the best condition for buffer deposition on the ECD counter electrode.

Ti:V2O5/ITO Films: Surface Roughness Properties
To understand the interfacial structure, the surface roughness of Ti:V2O5 counter electrodes on ITO glass was collected by AFM to investigate the film surface topography deposited with different Ar/O2 gas flow ratios (samples 1-4). Figure 5 shows the Ti:V2O5 film visualization of AFM in two dimensions (2D) and three dimensions (3D). In order to pre-

Ti:V 2 O 5 /ITO Films: Surface Roughness Properties
To understand the interfacial structure, the surface roughness of Ti:V 2 O 5 counter electrodes on ITO glass was collected by AFM to investigate the film surface topography deposited with different Ar/O 2 gas flow ratios (samples 1-4). Figure 5 shows the Ti:V 2 O 5 film visualization of AFM in two dimensions (2D) and three dimensions (3D). In order to present the images, a scan area of 1 × 1 µm 2 was used. The measurements of topographical parameters are listed in Table 3. This work focuses on fabricating Ti:V 2 O 5 films as a counter electrochromic layer by CAP deposition through four different oxygen and argon ratios. Here, we focus on how to fabricate nanostructure and surface roughness, so as to enhance fast ion insertion/extraction. According to the Thornton model [7,40], a loose-packed porous structure is formed under high-pressure environments. Arc discharge can be operated in high working pressure environments; interesting phenomena may occur such as self-organized synthesis of nanostructure and reduction in macroparticle size. When the arc is operated at higher working pressures, intense ion bombardment and ohmic heating likely allow a switch to thermionic mode; in this case, the erosion craters become smaller, facilitating the formation of a columnar structure. Figure 6 shows that Ar/O 2 gas flow ratio of 1/3 led to the smallest average roughness (Ra) 3.9 nm and the Ti:V 2 O 5 film surface was peak-shaped. In contrast with other ratios, the higher (1/3.5) or lower (1/2 and 1/2.5) Ar/O 2 gas flow ratios led to a higher average roughness (Ra). This result indicated that the smallest Ra was consistent with the cyclic voltammetry (CV) results for the Ar/O 2 gas flow ratio of 1/3 (sample 3), due to it having a larger enveloped area, which enables the particles to gain energy to migrate along the surface. The enveloped area of the CV curve correlated with the film surface topography. Under the electrochemical redox reaction of the Ti:V 2 O 5 film, the topography may have the crucial influence on the insertion/extraction of Li ions at the counter electrode.
The surface roughness of the electrode is an essential indicator for light scattering. As shown in Figure 6, the gas flow ratio of 1/3 for Ti:V 2 O 5 resulted in the highest optical transmittance (∆T = 27%), based on the smallest average roughness (Ra). The higher transmittance obtained might be ascribed to the reduction in light scattering [40]. The counter electrode surface deposited on the smallest Ra value could provide a prominent platform to insert the IrO 2 buffer layer for fabricating an ideal ECD.

IrO 2 Buffer/Ti:V 2 O 5 /ITO Films: Coloration Efficiency Analysis
Coloration efficiency (CE) is an imperative criterion for evaluating the assessment of electrochemical performance. It is defined as the change in optical density (∆OD) per unit insert charge Q in (Q in = Q/A, which is the charge (Q) per unit area (A) of the electrode film). The calculation can be formulated as follows: where T bleaching and T coloring are the transmittance values of the bleaching and coloring states at the specific wavelength of 633 nm, respectively. the topography may have the crucial influence on the insertion/extraction of Li ions at the counter electrode. The surface roughness of the electrode is an essential indicator for light scattering. As shown in Figure 6, the gas flow ratio of 1/3 for Ti:V2O5 resulted in the highest optical transmittance (∆T = 27%), based on the smallest average roughness (Ra). The higher transmittance obtained might be ascribed to the reduction in light scattering [40]. The counter electrode surface deposited on the smallest Ra value could provide a prominent platform to insert the IrO2 buffer layer for fabricating an ideal ECD. The optical transmittance spectra and CE value of Ti:V 2 O 5 film and IrO 2 buffer/Ti:V 2 O 5 /ITO film were determined for the gas flow ratio of 1/3 (sample 3).The amount of charge interca-lated (Q in ) when a negative potential is applied were was integrated by chronoamperometry (CA) measurement. A high CE value (cm 2 C −1 ) is achieved when a large change in optical density is driven by a low amount of inserted charge. In Figure 7a,b, the optical transmittance spectra of Ti:V 2 O 5 film and IrO 2 buffer/Ti:V 2 O 5 film with gradually applied successive potential voltages from +2.0 V (bleaching state) to −2.2 V (coloring state) during a pulsed time interval of 90 s are shown. The change in optical transmittance corresponds to the voltage between the lowest transmittance in the coloring state (T coloring ) and the highest transmittance in the bleaching state (T bleaching ). The two electrode films were subjected to gradually decreasing voltages in accordance with the decreasing transmittance. The ∆OD value was nearly linear. The coloring/bleaching states were determined by the positive/negative voltage. IrO 2 buffer/Ti:V 2 O 5 film demonstrated lower transmittance than the Ti:V 2 O 5 film at the coloring state due to inserting a buffer.  Figure 7c,d shows the optical density change vs. charge density of Ti:V2O5 films and IrO2 buffer/Ti:V2O5 films. The higher CE values indicate that electrodes can provide large optical modulation with small quantities of Li + intercalation/extraction [40,41]. The CE value is calculated from the slope of the line fitted to the linear region of the curve. Compared with the two curves, the CE value of the IrO2/Ti:V2O5 film (96.1 cm 2 /C) is significantly higher than that of the Ti:V2O5 film (33.1 cm 2 /C). The Ti:V2O5 film with an IrO2 buffer layer provided a higher CE value and is good for promoting optical transmittance.  Figure 8a,b shows X-ray diffraction (XRD) of Ti:V2O5 films and IrO2 buffer/Ti:V2O5 film at an Ar/O2 ratio of 1/3. X-ray diffraction was used to assess the crystalline structure and phase in the scanning range from 20° to 90°. To determine the standard pattern identification, use was made of the Joint Committee on Powder Diffraction Standard (JCDPS).   [40,41]. The CE value is calculated from the slope of the line fitted to the linear region of the curve. Compared with the two curves, the CE value of the IrO 2 /Ti:V 2 O 5 film (96.1 cm 2 /C) is sig-nificantly higher than that of the Ti:V 2 O 5 film (33.1 cm 2 /C). The Ti:V 2 O 5 film with an IrO 2 buffer layer provided a higher CE value and is good for promoting optical transmittance. Figure 8a,b shows X-ray diffraction (XRD) of Ti:V 2 O 5 films and IrO 2 buffer/Ti:V 2 O 5 film at an Ar/O 2 ratio of 1/3. X-ray diffraction was used to assess the crystalline structure and phase in the scanning range from 20 • to 90 • . To determine the standard pattern identification, use was made of the Joint Committee on Powder Diffraction Standard (JCDPS). Figure 8b, the IrO2 buffer/Ti:V2O5 film can obtain higher optical transmittance ∆T (from Tbleaching to Tcoloring) than the Ti:V2O5 film (Figure 8a). The crystallinity characteristic of the counter electrode films is closely associated with their transmittance.

crystallinity. As shown in
The vibrations measured in Raman spectroscopy are determined by material structure shown in Figure 8c. Raman spectra of the Ti:V2O5 films produced by various Ar/O2 gas flow ratios (1/2, 1/2.5, 1/3 and 1/3.5) in the wavelength range of 500 cm −1 to 2000 cm −1 are shown. We found that, with an Ar/O2 gas flow ratio of 1/3, the Ti:V2O5 film exhibits a clearer and more intense band at 673 cm −1 and broader bands at 945 cm −1 , 1090 cm −1 , and 1245 cm −1 compared to other ratios, which have uncharacteristic Raman spectra. However, in comparison with Figure 8d, the IrO2 buffer/Ti:V2O5 film (Ar/O2 gas flow ratio of 1/3) has a distinguishable sharp band at 1406 cm −1 and broad bands at 1390 cm −1 and 1156 cm −1 , corresponding to the crystalline preferential orientation of (101) in Figure 8b. After inserting the buffer in the Ti:V2O5 films (Ar/O2 gas flow ratio of 1/3), these bands disappeared.   Figure 8a shows that the XRD spectrum of Ti:V 2 O 5 films (Ar/O 2 ratio of 1/3) lacked the main peak, which indicates that the film could be an amorphous structure. The characteristics of the Ti:V 2 O 5 films were not found in the XRD pattern. Figure 8b shows the XRD spectrum of the IrO 2 buffer/Ti:V 2 O 5 film. The most intense diffraction peak was located at a 2θ angle of 34 • (JCPDS card no. 47-1049) and corresponded to a preferential orientation of (101), which stacked along the c-axis. As our report investigates the influence of inserting the buffer, it can be observed that the use of IrO 2 as a buffer on the Ti:V 2 O 5 film (Ar/O 2 ratio of 1/3) is an effective way to improve the crystallinity. As shown in Figure 8b, the IrO 2 buffer/Ti:V 2 O 5 film can obtain higher optical transmittance ∆T (from T bleaching to T coloring ) than the Ti:V 2 O 5 film (Figure 8a). The crystallinity characteristic of the counter electrode films is closely associated with their transmittance. The vibrations measured in Raman spectroscopy are determined by material structure shown in Figure 8c. Raman spectra of the Ti:V 2 O 5 films produced by various Ar/O 2 gas flow ratios (1/2, 1/2.5, 1/3 and 1/3.5) in the wavelength range of 500 cm −1 to 2000 cm −1 are shown. We found that, with an Ar/O 2 gas flow ratio of 1/3, the Ti:V 2 O 5 film exhibits a clearer and more intense band at 673 cm −1 and broader bands at 945 cm −1 , 1090 cm −1 , and 1245 cm −1 compared to other ratios, which have uncharacteristic Raman spectra. However, in comparison with Figure 8d, the IrO 2 buffer/Ti:V 2 O 5 film (Ar/O 2 gas flow ratio of 1/3) has a distinguishable sharp band at 1406 cm −1 and broad bands at 1390 cm −1 and 1156 cm −1 , corresponding to the crystalline preferential orientation of (101) in Figure 8b. After inserting the buffer in the Ti:V 2 O 5 films (Ar/O 2 gas flow ratio of 1/3), these bands disappeared.  Figure 9b,c compares the surface morphology of the two materials. Figure 9b shows a Ti:V 2 O 5 /ITO film at an Ar/O 2 gas flow ratio of 1/3. This is a featureless structure with a smooth and uneven, flakey surface. It might be related to the amorphous structure in Figure 8a imaged by XRD spectroscopy.  Figure 9a shows the cross-section morphology of the IrO2 buffer/Ti:V2O5 film at an Ar/O2 gas flow ratio of 1/3. The 100 nm electrode thickness includes IrO2 buffer of 20 nm and Ti:V2O5 film of 80 nm. The IrO2 buffer/Ti:V2O5 is stacked on indium tin oxide (ITO) glass substrate with a thickness of 300 nm. Figure 9b,c compares the surface morphology of the two materials. Figure 9b shows a Ti:V2O5/ITO film at an Ar/O2 gas flow ratio of 1/3. This is a featureless structure with a smooth and uneven, flakey surface. It might be related to the amorphous structure in Figure 8a imaged by XRD spectroscopy.

IrO2 Buffer/Ti:V2O5/ITO Films: Surface Morphology
In Figure 9c, the IrO2 buffer on the Ti:V2O5 film at an Ar/O2 ratio of 1/3 is shown. It has a filamentary and interconnected structure. The morphological result is identical to our previous research [38]. As we found previously, this type of structure is useful for the transfer of Li ions in/out of the interface of the electrode due to the morphology, which possesses a larger inner pore that furnishes a great contact area and abundant porosity. This also proved that the filamentary and interconnected type of structure exhibits higher optical transmittance in Figure 7b and CE value (96.1 cm 2 /C) in Figure 7d of the IrO2 buffer/Ti:V2O5 film than optical transmittance in Figure 7a and CE value (33.9 cm 2 /C) in Figure 7b of the Ti:V2O5 film.  Figure 10 demonstrates the optical transmittance spectra comparison with buffered ECD and without buffered ECD at bleaching/coloring state, based on the continuous potential voltage 2.5 V to −3 V. For the buffered ECD (glass/ITO/WO3/liquid electrolyte/IrO2 buffer/Ti:V2O5(Ar/O2 ratio 1/3)/ITO/glass), the optical transmittance modulation was ∆T = In Figure 9c, the IrO 2 buffer on the Ti:V 2 O 5 film at an Ar/O 2 ratio of 1/3 is shown. It has a filamentary and interconnected structure. The morphological result is identical to our previous research [38]. As we found previously, this type of structure is useful for the transfer of Li ions in/out of the interface of the electrode due to the morphology, which possesses a larger inner pore that furnishes a great contact area and abundant porosity. This also proved that the filamentary and interconnected type of structure exhibits higher optical transmittance in Figure 7b and CE value (96.1 cm 2 /C) in Figure 7d of the IrO 2 buffer/Ti:V 2 O 5 film than optical transmittance in Figure 7a and CE value (33.9 cm 2 /C) in Figure 7b of the Ti:V 2 O 5 film.

Buffer ECD: Optical Transmittance and Durability
3.6. Buffer ECD: Optical Transmittance and Durability Figure 10 demonstrates the optical transmittance spectra comparison with buffered ECD and without buffered ECD at bleaching/coloring state, based on the continuous potential voltage 2.5 V to −3 V. For the buffered ECD (glass/ITO/WO 3 /liquid electrolyte/IrO 2 buffer/Ti:V 2 O 5 (Ar/O 2 ratio 1/3)/ITO/glass), the optical transmittance modulation was ∆T = 57% (from T bleaching (67%) to T coloring (10%)) at 633 nm, in the range from 300 nm to 1000 nm, which was higher than without the buffer (ITO/WO 3 /liquid electrolyte/Ti:V 2 O 5 (Ar/O 2 ratio 1/3)/ITO) (∆T = 36% (from T bleaching (58%) to T coloring (22%)). This could be attributed to a larger CV enveloped area for the buffered-ECD, as shown in Figure 11, on account of the film with greater Li + intercalation/extraction as shown by optical transmittance during the CV analysis. Remarkably, this result was in good agreement with Figure 3, in which the largest CV enveloped area demonstrated the highest transmittance.

5179
13 of 17 57% (from Tbleaching (67%) to Tcoloring (10%)) at 633 nm, in the range from 300 nm to 1000 nm, which was higher than without the buffer (ITO/WO3/liquid electrolyte/Ti:V2O5 (Ar/O2 ratio 1/3)/ITO) (∆T = 36% (from Tbleaching (58%) to Tcoloring (22%)). This could be attributed to a larger CV enveloped area for the buffered-ECD, as shown in Figure 11, on account of the film with greater Li + intercalation/extraction as shown by optical transmittance during the CV analysis. Remarkably, this result was in good agreement with Figure 3, in which the largest CV enveloped area demonstrated the highest transmittance. The durability of the ECD is an important factor to determine whether the product can work in real life. Figure 12a presents the long-life (1000 cycles) durability comparison between the buffered ECD and the ECD without buffer. After 1000 cycles of bleaching/coloring, the buffered ECD had notable durability, retaining 98% (i.e., 2% decay) of the initial value, greater than 78% (22% decay) for the ECD without buffer. The high-contrast optical performance and good durability of the ECD could be attributed to the inserted IrO2 buffer on the electrode. We found that both optical transmittance and durability were, in terms of electrode surface morphology, equipped with filamentary and interconnect type structure. The buffer ECD with the IrO2 buffer/Ti:V2O5 electrode provided a higher CE value (96.1 cm 2 /C) to support the Li + intercalation/extraction process. Figure 12b,c illustrates the buffered ECD and the ECD without buffer; after insertion of the buffer, the switching response time was from 1.4 s in the bleaching state to 4.0 s in the coloring state, which was faster than the ECD without buffer (response time was from 1.5 s in the bleaching state to 5.2 s in the coloring state). In addition, we also survey the comparison of recent research on electrodes under various conditions in Table 4.    The durability of the ECD is an important factor to determine whether the product can work in real life. Figure 12a presents the long-life (1000 cycles) durability comparison between the buffered ECD and the ECD without buffer. After 1000 cycles of bleaching/coloring, the buffered ECD had notable durability, retaining 98% (i.e., 2% decay) of the initial value, greater than 78% (22% decay) for the ECD without buffer. The high-contrast optical performance and good durability of the ECD could be attributed to the inserted IrO 2 buffer on the electrode. We found that both optical transmittance and durability were, in terms of electrode surface morphology, equipped with filamentary and interconnect type structure. The buffer ECD with the IrO 2 buffer/Ti:V 2 O 5 electrode provided a higher CE value (96.1 cm 2 /C) to support the Li + intercalation/extraction process. Figure 12b,c illustrates the buffered ECD and the ECD without buffer; after insertion of the buffer, the switching response time was from 1.4 s in the bleaching state to 4.0 s in the coloring state, which was faster than the ECD without buffer (response time was from 1.5 s in the bleaching state to 5.2 s in the coloring state). In addition, we also survey the comparison of recent research on electrodes under various conditions in Table 4.   Figure 11. The CV curve comparison between buffered ECD and ECD without buffer.

Conclusions
We established an appropriate electrode, Ti:V 2 O 5 , as a base to insert a buffer. According to our results, the buffer inserted on the Ti:V 2 O 5 electrode film with exclusive surface morphology not only effectively increased the coloration efficiency (CE), but also promoted optical transmittance and durability. Moreover, strategies such as Ti:V 2 O 5 films are based on a series of Ar/O 2 gas flow ratios (1/2, 1/2.5, 1/3, and 1/3.5) on indium tin oxide (ITO) glass to establish the appropriate electrode.
Subsequently, we picked the Ti:V 2 O 5 film with an Ar/O 2 gas flow ratio of 1/3 as the best electrode base. This film had the largest cyclic voltammetry (CV) area to allow more Li ions into/out of the electrode interface and presented the highest optical transmittance (∆T) of 27%. Atomic force microscopy (AFM) was performed to obtain a deep understanding of the surface topography of the electrode interface. In addition, this value of Ti:V 2 O 5 (Ar/O 2 = 1/3) is helpful for optical transmittance, as it possesses the smallest average roughness (Ra = 3.53 nm) to reduce light scattering.
To distinguish the difference when the buffer was inserted on the electrode, we implemented many analyses. Regarding coloration efficiency (CE), the IrO 2 buffer/Ti:V 2 O 5 film achieved a higher value (96.1 cm 2 /C), providing large optical modulation, than the Ti:V 2 O 5 film without buffer (33.9 cm 2 /C). Regarding crystallinity, the IrO 2 buffer/Ti:V 2 O 5 film, which has an intense diffraction peak at a 2θ angle of 34 • and a preferential orientation of (101), is better than the Ti:V 2 O 5 film, which has an amorphous structure. Regarding surface morphology, the IrO 2 buffer/Ti:V 2 O 5 film with a filamentary and interconnected structure, which provides larger inner pore and contact area, improves Li ion transfer in/out interface of the electrode compared with the Ti:V 2 O 5 film with a featureless structure.
We successfully fabricated a buffered ECD via a vacuum cathodic arc plasma (CAP) technique. Our goal was to insert the IrO 2 buffer to enhance the properties of the ECDs. Compared to the ECD without buffer, the buffered ECD promoted optical transmittance modulation (∆T = 57%) and maintained excellent durability of up to 98% (2% decay). This may provide a new insight into the development of energy devices. The superior electrochromic performance with the buffer layer makes our ECD a prominent candidate for use in smart windows with reduced energy demand.